Abstract
The Rashba effect plays important roles in emerging quantum materials physics and potential spintronic applications, entailing both the spin orbit interaction (SOI) and broken inversion symmetry. In this work, we devise asymmetric oxide heterostructures of LaAlO_{3}//SrTiO_{3}/LaAlO_{3} (LAO//STO/LAO) to study the Rashba effect in STO with an initial centrosymmetric structure, and broken inversion symmetry is created by the inequivalent bottom and top interfaces due to their opposite polar discontinuities. Furthermore, we report the observation of a transition from the cubic Rashba effect to the coexistence of linear and cubic Rashba effects in the oxide heterostructures, which is controlled by the filling of Ti orbitals. Such asymmetric oxide heterostructures with initially centrosymmetric materials provide a general strategy for tuning the Rashba SOI in artificial quantum materials.
Introduction
Manipulation of the spin degree of freedom can be expanded to various nonmagnetic materials by the Rashba effect, where both the spin–orbit interaction (SOI) and broken inversion symmetry are required^{1,2,3,4}. The phenomenon is generally observed at the surface of heavy metals and in asymmetric twodimensional quantum wells, where the inversion symmetry is broken naturally^{3,5}. Since the Rashba effect plays a key role not only in fundamental physics but also for potential applications, there has been considerable effort devoted to exploring and/or maximizing the Rashba effect in a wide range of materials^{6}. In principle, an external electric field can break and tune the inversion symmetry of the materials studied^{7,8}, which is also the mechanism of the celebrated spin transistor^{9}. However, such a technique is limited by the magnitude and the screening length it can achieve^{10,11,12}. As a result, much attention has been paid to exploring structures with intrinsically broken inversion symmetry, such as ferroelectrics and polar semiconductors^{13,14,15,16}. Recently, the effort has been extended to manipulate the geometric environment of orbitals to achieve a giant Rashba effect^{6,17,18}.
Complex perovskite oxides ABO_{3} show great potential for exploiting the Rashba effect^{6,19} because their multiple degrees of freedom, i.e., charge, spin, orbital, and lattice, are entangled with one another^{20,21}. In heterostructures of perovskite oxides ABO_{3} and A'B'O_{3}, two different interfaces, i.e., AOB'O_{2} and BO_{2}A'O, in the [001] direction can be introduced^{22,23}. SrTiO_{3} (STO), which has 3d electrons, is a prototypical example (Fig. 1a). However, there is no spin splitting in the 3d electron band for the centrosymmetric STO, and strain and SOI can lift the degeneracy of only the 3d orbitals (Fig. 1b). Spin splitting requires breaking the inversion symmetry of the structure, for example, when STO forms a heterointerface with (LaO)^{+} interface due to the polar discontinuity of LAO^{23,24,25,26,27}. Such a significant Rashba effect in the system has led to the discovery of significant spin–charge conversions^{28,29,30} and the perspective of various exotic properties, such as skyrmion^{31,32}, topological superconductivity^{33}, and intrinsic spin Hall effect^{34}. In this heterostructure, the inversion symmetry at the interface is naturally broken, and the band structure is significantly modified owing to the confinement effect and other interfacerelated effects^{20,22}.
As illustrated in Fig. 1a (right), we propose in this work that broken inversion symmetry can be manipulated by creating two unequal interfaces in LAO//STO/LAO oxide heterostructures, which makes use of their opposite polar discontinuities, i.e., (AlO_{2})^{−}(SrO) versus (TiO_{2})(LaO)^{+}. In this scheme, the potential difference between these two unequal interfaces produces a builtin electric field to break the inversion symmetry of STO^{35}. Compared to the wellstudied LAO/STO heterostructure (Supplementary Figs. 1 and 2), where the inversion symmetry is naturally broken at the interface, this designed approach is capable of modulating the broken inversion symmetry via tuning the intermediate STO layer thickness. Combining density functional theory (DFT)based tightbinding calculations with weak antilocalization (WAL) measurements, the transition from the pure cubic Rashba term to its coexistence with the linear term is identified as a function of carrier filling in Ti orbitals. Our work demonstrates a general platform for exploring Rashba SOI physics in interfaceasymmetric heterostructures with initially centrosymmetric materials.
Results
Tuning of Rashba effect in the LAO//STO/LAO heterostructures
The band structure of STO with a centrosymmetric structure and compressive strain from LAO was obtained from DFTbased tightbinding calculation (Fig. 1b). Owing to the biaxial strain in the (001) plane, the degeneracy of Ti t_{2g} is lifted with the d_{xy} orbital located above the d_{yz/xz} orbitals. When considering the SOI, the degeneracy of the d_{yz/xz} band is further lifted. Nevertheless, owing to the inversion symmetry of STO, the energy band is doubly degenerate in the entire Brillouin zone, which does not result in spin splitting (indicated by the green arrows in Fig. 1b). As proposed above, the feature can be achieved by introducing two unequal interfaces between LAO and STO, which breaks the inversion symmetry of STO, as confirmed by our calculation (Fig. 1c). The resulting Rashba effect lifts the double degeneracy of the energy band away from the Γ point, i.e., resulting in spin splitting of the 3d orbitals (green arrows in Fig. 1c).
Furthermore, the linear and cubic Rashba terms, where the spin splitting is linearly and cubically proportional to the momentum k (inset of Fig. 1d), respectively, are predicted to coexist in the t_{2g} multiorbitals. These two types of Rashba effects result in different spin configurations in each Fermi surface and may further lead to different spinrelated properties^{36,37,38}. Importantly, the characteristics of the Rashba effect can be controlled by the filling of carriers at the Ti sites. Figure 1d shows the spin splitting energy as a function of the carrier concentration at each Ti atom for the cubic and linear Rashba effects. In the STO with inversion symmetry broken, the linear Rashba effect emerges when the carrier concentration reaches approximately 0.01 e/Ti. We should note that this critical carrier concentration is an intrinsic property of STO and determined by its electronic band structure. We hypothesize that the asymmetric interfaces of the LAO//STO/LAO structures can be validated by characterizing the Rashba effect, which might be tuned by the carrier concentration in the STO layers. Such asymmetric multilayers consisting of initially centrosymmetric materials provide a general platform for investigating the Rashba SOI in engineered heterostructures.
It is important to note that, although the existence of the linear Rashba effect was theoretically predicted in oxide herterostructures with Ti 3d electrons^{38,39,40}, so far only the cubic Rashba effect has been reported in transport studies^{25,41,42}. One possible explanation is that the electrons from the d_{xy} orbital are localized at the interface and do not contribute to charge transport^{43}. In this work, we envision that the itinerant nature of the electrons in the asymmetric LAO//STO/LAO heterostructures will enable us to explore the linear Rashba effect and its coexistence with the cubic Rashba effect will be modulated via carrier filling in Ti orbitals.
Heterostructure synthesis and scanning transmission electron microscopy (STEM) characterization
The oxide heterostructures were grown on treated LAO substrates using pulsed laser deposition (PLD). The thickness and the termination of the LAO and STO layers are precisely controlled via monitoring reflection highenergy electron diffraction (RHEED) (see Supplementary Fig. 4a for a typical heterostructure with 15 uc STO). As discussed in the previous section, as a result of the polar nature of LAO, such oxide heterostructures are designed to be asymmetric: the (AlO_{2})^{−}–SrO interface between the LAO substrate and the STO layer is presumably p type^{23,44}, while the top TiO_{2}–(LaO)^{+} interface is n type. However, as we will discuss below, factors like cation intermixing at the interfaces make the actual heterostructure deviate from the design although the asymmetric nature is retained.
To confirm the high quality of the films, Xray reflectivity experiments were conducted, and a typical result is shown in Supplementary Fig. 4b. From the simulation of the reflectivity data, we derived the thicknesses of each layer in the heterostructure, which are consistent with the RHEED results. By fitting the fringe oscillations of the highresolution Xray theta2theta measurements, we extracted the outofplane c lattice parameter of the STO layer. Interestingly, it was found that c decreases from 3.946 to 3.895 Å when the STO thickness decreases in the series of heterostructures (see Supplementary Fig. 4d). Such a feature is ascribed to the electrostriction effect due to the builtin electric field^{45}, which is supported by our DFT calculations (see Supplementary Note 3).
To further characterize the strain state of the STO layer and, especially, the interface atomic structures, aberrationcorrected STEM was used. A typical LAO//STO/LAO structure with 20 uc STO was characterized. As shown by the highangle annular darkfield (HAADF)STEM images in Fig. 2, epitaxial and coherent growth of the STO layer is confirmed. The crosssection HAADFSTEM image of the LAO//STO/LAO heterostructure and the strain components parallel (ε_{xx}) and perpendicular (ε_{yy}) to the interface are presented in Supplementary Fig. 5, which further supports the coherent growth of the heterostructure. Crosssectional elemental mapping was also obtained by atomically resolved STEMenergydispersive Xray spectroscopy, from which we can acquire information on the local composition around the interfaces in such heterostructures. Similar to reports on the STO/LAO interface^{44,46,47}, cation intermixing was observed at both interfaces in the LAO//STO/LAO heterostructure. More importantly, we found that the intermixing of the top and bottom interfaces are different; it spans approximately 1 uc for the bottom interface and 2 uc for the top interface, as indicated in the overlay images in Fig. 2. This variation in the cation mixing has been discussed as one of the key differences of ntype and ptype interfaces^{44}. It should be noted that the cation intermixing at the bottom interface results in a combination of (AlO_{2})^{−}SrO and (LaO)^{+}TiO_{2} configurations. This atomic reconstruction can be regarded as a response to the polar discontinuity due to an energy gain compared to that from generating the holedoped interface, which was reported in other similar oxide heterostructures^{48,49}. Although the atomic structures of the interfaces deviate from the ideal case (Fig. 1a), the LAO//STO/LAO heterostructure remains asymmetric.
Thicknessdependent density of 3d electrons
Hall effect measurements were performed to obtain the carrier density of the LAO//STO/LAO heterostructures. Figure 3a shows the typical Hall measurements for the structure with 8, 20, and 30 uc STO, from which the sheet carrier density was calculated. It was found that the sheet carrier concentration (n_{H}) increased progressively from 1.07 × 10^{14} to 1.92 × 10^{14} cm^{−2} with decreasing STO layer thickness, as shown in Fig. 3b. It is important to note that the carrier concentration is higher in the heterostructures with thinner STO layers. The corresponding averagedfilling electrons per Ti in the heterostructure exhibits a similar trend as a function of the STO thickness (inset of Fig. 3b). In the rough estimation, the carriers are assumed to be homogeneously doped in the entire STO layer, which does not reflect the local deviation of the electron filling across the STO layer. As expected from the designed LAO/STO/LAO structure with two nonequivalent interfaces, the electron distribution across the whole STO layer should show a gradual increase from the ptype interface to the ntype interface. Furthermore, the localized electrons near the interfaces may have an important influence on the internal electric field and impact on the Rashba splitting. Nevertheless, the carrier density estimated from the Hall effect measurement exhibits a consistent trend of dependence on the STO layer thickness. When the STO layer in the heterostructure increases from 8 uc to 60 uc, the number of electrons per Ti decreases from 0.038 to 0.003. This range of electron filling is smaller than that in the extensively investigated LAO/STO structures where the induced electrons are mainly located around the interface.
In such heterostructures, both the electrons due to the polar LAO layer and those doped by the defects introduced during growth may contribute to the conduction. If the carriers were introduced mainly by the growthrelated defects, the sheet carrier concentration (n_{s}) with a bulk origin would increase with the STO thickness, which is opposite to our observation (inset of Fig. 3b). Thus defects are not the dominant source of conducting carriers. Furthermore, a control experiment was conducted on a heterostructure with amorphous La_{0.7}Sr_{0.3}MnO_{3} (aLSMO) as the capping layer, i.e., LAO/STO/aLSMO, which was prepared under the same conditions as the LAO//STO/LAO heterostructures except that the top LSMO layer was deposited at room temperature. The absence of measurable conductivity in such a LAO//STO/aLSMO structure indicates that the polarity of the LAO plays an essential role in introducing the itinerant carriers^{35}, which may be achieved by influencing the formation energy of the oxygen vacancy.
Evolution of SOI in LAO//STO/LAO heterostructures
As quantum corrections to the conductance, both weak localization (WL) and WAL can be present at low temperatures in oxide heterostructures. Because these effects are sensitive to an external magnetic field, magnetotransport measurements can provide insights into the nature of SOI^{50}. Figure 4 shows the magnetoresistance (MR) of a heterostructure with 30 uc STO inserted between the LAO layers. The negative MR at 20 and 30 K is a signature of WL, while with decreasing temperature, a cusp emerges around the zero field and broadens progressively. Such MR features at low temperatures are manifestations of WAL and are indicative of the presence of a strong SOI in the systems^{25,41}.
By varying the thickness of the STO layer in the heterostructures, magnetotransport of the LAO//STO/LAO heterostructures can be systemically tuned. As shown for the 2 K MR data in Fig. 5a, the zerofield cusp shrinks with increasing STO layer thickness, and finally, a negative MR emerges with the high magnetic field at the thickest STO layer of 60 uc. This indicates a crossover from the WAL to the WL regime with increasing STO thickness. In the WL, the phase coherence of itinerant electrons is destroyed mainly by inelastic scattering^{50}, while the WAL is governed by SOI. Thus the change in the MR characteristics upon changing the thickness of the STO layer reflects a significant modulation of the SOI in the heterostructures^{24,25,42,51}.
To quantify the modulation of SOI upon the change of STO layer thickness, the model developed by Iordanskii, LyandaGeller, and Pikus (ILP), which considers the kdependent SOI, was adopted to analyze the magnetotransport data^{52,53}. This model involves two spinsplitting energy terms due to different kdependent spinprecession vectors, i.e., one is the linear SOI term and the other is the cubic SOI term. The full equation of the ILP model can be written as follows:^{52}
where
In the equation, B_{so1}, B_{so3}, and B_{φ} refer to the characteristic effective magnetic fields for the linear SOI, the cubic SOI, and the phase coherence, respectively, and Ψ is the digamma function. Here the diffusion limit of this model is satisfied as the applied magnetic field is much smaller than the B_{e}, the characteristic field of the elastic scattering, which is of the order of 100 T because of the short mean free path in our heterostructures. To account for the classical Lorentz force, which manifests itself as quadratic dependence in field, the resistivity data are fitted directly using
where α is the coefficient for the MR due to the Lorentz force, γ is a constant, ln(2)/π, due to the Van der Pauw method used for the transport measurements, and δ is the fieldindependent component of conductivity of the samples. The data were symmetrized to avoid any artifact due to the choice of magnetic field direction. The analysis of the fitting accuracy can be found in Supplementary Fig. 6. Compared to the fitting with only a cubic SOI term, the fitting considering both linear and cubic SOI terms gives a more accurate result.
Figure 5b shows the fitting result of the magnetoconductance data using the ILP model, which are obtained after removing the classical Lorentz components, and the derived fitting parameters are shown in Fig. 5c. One main finding of this work is that B_{so3} monotonically increases from 1 to 3.75 T as the thickness of the STO layer decreases from 60 uc to 8 uc in the LAO//STO/LAO heterostructures. The sampledependent B_{φ} fluctuates in the range of 1–2 T, which is smaller than the characteristic B_{so3} and thus in line with the WAL mechanism^{50}. More significantly, B_{so1} emerges only when the thickness of the STO layer is below 20 uc; it monotonically increases to 2.13 T in the thinnest heterostructure with 8 uc STO. The temperaturedependent characteristic fields have been extracted too, as shown in Supplementary Fig. 7. Our data indicate that the prerequisite of the emergence of the linear Rashba SOI is a high doping level of 3d electrons in thin STO layers. On the other hand, the cubic SOI was found to dominate in the heterostructures with STO thickness above 20 uc, similar to the recent report by Nakamura et al.^{41}. The temperaturedependent resistance for all the samples are shown in Supplementary Fig. 8, where an upturn behavior of resistance was observed at low temperatures. Furthermore, the Xray linear dichroism (XLD) experiments has been performed to confirm that the lowest orbital in the LAO//STO/LAO structure is d_{xz/yz} and the electron occupation changes upon the thickness of the STO layer (Supplementary Note 5 and Fig. 9). The XLD result strongly supports the scenario that the Rashba effect is tuned in the LAO//STO/LAO structures by carrier filling of the Ti 3d orbitals.
Accordingly, the thickness dependence of spin diffusion lengths due to the linear and cubic SOI terms was calculated using the equation \(l_{{\mathrm{so}}} = \sqrt {\hbar /4eB_{{\mathrm{so}}}}\)^{50}. As described in Supplementary Note 6, we calculated the linear Rashba coefficient α_{linear} and the spin splitting energy Δ_{cubic} from the cubic SOI term for the heterostructures. The linear Rashba coefficient increases from 0.015 to 0.043 eVÅ upon a decrease in the STO layer thickness from 15 uc to 8 uc, which is in the same range as the results of recent reports^{25,40}. When the thickness of the STO layer decreases from 60 uc to 20 uc, the spin splitting energy due to the cubic SOI term increases from 2.31 to 2.87 meV, and concurrently the electron number per Ti increases from 0.003 to 0.01. The measured spin splitting energy is consistent with the firstprinciples calculation result (Fig. 1d). To elucidate the relationship between the SOI transition and the electron doping level of Ti, we plotted the above extracted parameters as functions of the filling electrons per Ti determined from the Hall measurement, as presented in Fig. 5d. It can be seen that the transition between the linear and cubic Rashba SOI occurs at a doping level of approximately 0.01–0.015 e/Ti, which is consistent with the value predicted by our firstprinciples calculation result.
In conclusion, we demonstrated a class of oxide heterostructures with interfacebased broken inversion symmetry, in which the Rashba effect can be tuned by changing the thickness of the intermediate layer with itinerant 3d electrons. The lifted orbital degeneracy and carriers’ doping modulated by the STO layer thickness in the LAO//STO/LAO heterostructures enabled us to identify the transition between the cubic and linear Rashba effects. This work offers an alternative heterostructurebased route to manipulating the SOI, complimentary to the reports on electric field effect. Furthermore, our study also reveals the unambiguous role of the linear Rashba SOI in thin heterostructures, while the previous reports were focused on cubic SOI at oxide interfaces. The coexistence of the linear and cubic Rashba effects in such oxide heterostructures with 3d electrons will stimulate further theoretical and experimental studies. Such asymmetric heterostructures represent an alternative platform for exploring SOI and other exotic physics in artificial quantum materials.
Methods
DFTbased tightbinding calculations
To construct a realistic tightbinding model for STObased heterostructure and also avoid adjustable parameters, we performed a projection^{54} of Wien2K^{55} DFT results for bulk STO onto maximally localized Wannier orbitals, which exactly reproduced the DFTcalculated band structure^{40,56}. The tightbinding Hamiltonian is described by H_{o} + H_{ξ} + H_{γ} in the t_{2g}(xy, yz, xz) basis. The H_{o} term contains local energy terms ε and hopping terms t. In bulk STO with cubic symmetry ε_{xy} = ε_{yz/xz}, which is defined with respect to Fermi energy level, the compressive strain from the LAO substrate increases the xy orbital energy in the order of 10 meV. Without loss of generality, we set ε_{xy} − ε_{xy/xz} = 20 meV. There are three hopping terms: the large hopping term of t_{1} = 0.277 eV arises from the large xy intraorbital hopping integral along the x and y directions; t_{2} = 0.031 eV and t_{3} = 0.076 eV indicate a much smaller hopping integral along the z and (1,1,0) directions of the xy orbital, respectively. The H_{ξ} term includes atomic SOI, whose strength is 19.2 meV, as estimated from the DFT calculated orbital splitting at Γ point. The last term H_{γ} = <xyHyz/xz> is an antisymmetric hopping between xy and yz/xz orbitals along the x/y direction. It describes the asymmetry due to the builtin electric field, which results in the Rashba spin splitting. In the bulk STO, H_{γ} vanishes due to inversion symmetry, while at the LAO/STO interface H_{γ} is 20 meV. It is noted that the Rashba transition as well as the corresponding critical carrier concentration mainly depend on H_{ξ} and the t_{2g} band structure character of STO. It is confirmed that a change of hopping terms t or crystal field splitting will not influence our conclusion.
Sample preparation and characterization
To ensure the AlO_{2} termination of the LAO substrate, all the substrates used were treated and confirmed by atomic force microscopic mapping before growth. The LAO//STO/LAO heterostructures were grown in a PLD system, and highpressure RHEED was used to monitor the growth quality and to control the thickness of the growing films. Both LAO and STO layers were grown at 800 °C under a pressure of 1 × 10^{−6} mbar of O_{2} and with the laser energy set at 1 J cm^{−2}. The laser pulse was set at a 1Hz repetition rate. After deposition, the samples were cooled to room temperature at 5 °C min^{−1}. With the same growth conditions, a series of heterostructures with controlled STO thicknesses were prepared. Van der Pauw method was used to perform the transport measurements with Ti/Au as the electrodes. All the transport measurements were conducted in a physical property measurement system (PPMS, Quantum Design). STEM was performed using a JEOL ARM200F operating at 200 kV and equipped with ASCOR probe corrector and Oxford XXMax 100TLE Xray detector.
Data availability
The data that support the findings of this study are available from the corresponding author upon reasonable request.
References
 1.
Winkler, R. Spin  Orbit Coupling Effects in Twodimensional Electron and Hole Systems (Springer Tracts in Modern Physics, Vol. 191) (SpringerVerlag, Berlin, Heidelberg, 2003).
 2.
Manchon, A., Koo, H. C., Nitta, J., Frolov, S. M. & Duine, R. A. New perspectives for Rashba spinorbit coupling. Nat. Mater. 14, 871–882 (2015).
 3.
Soumyanarayanan, A., Reyren, N., Fert, A. & Panagopoulos, C. Emergent phenomena induced by spin–orbit coupling at surfaces and interfaces. Nature 539, 509–517 (2016).
 4.
Yu, A. B. & Rashba, E. I. Oscillatory effects and the magnetic susceptibility of carriers in inversion layers. J. Phys. Condens. Matter 17, 6039–6045 (1984).
 5.
Zhang, X., Liu, Q., Luo, J.W., Freeman, A. J. & Zunger, A. Hidden spin polarization in inversionsymmetric bulk crystals. Nat. Phys. 10, 387–393 (2014).
 6.
Sunko, V. et al. Maximal Rashbalike spin splitting via kineticenergycoupled inversionsymmetry breaking. Nature 549, 492–496 (2017).
 7.
Nitta, J., Akazaki, T., Takayanagi, H. & Enoki, T. Gate control of spinorbit interaction in an inverted In_{0.53}Ga_{0.47}As/In_{0.52}Al_{0.48}As heterostructure. Phys. Rev. Lett. 78, 1335–1338 (1997).
 8.
Lin, W.N. et al. Electrostatic modulation of LaAlO_{3}/SrTiO_{3} interface transport in an electric doublelayer transistor. Adv. Mater. Interfaces 1, 1300001 (2014).
 9.
Datta, S. & Das, B. Electronic analog of the electro‐optic modulator. Appl. Phys. Lett. 56, 665–667 (1990).
 10.
Petersen, L. & Hedegård, P. A simple tightbinding model of spin–orbit splitting of spderived surface states. Surf. Sci. 459, 49–56 (2000).
 11.
Ahn, C. H., Triscone, J. M. & Mannhart, J. Electric field effect in correlated oxide systems. Nature 424, 1015–1018 (2003).
 12.
Song, C., Cui, B., Li, F., Zhou, X. & Pan, F. Recent progress in voltage control of magnetism: Materials, mechanisms, and performance. Prog. Mater. Sci. 87, 33–82 (2017).
 13.
Di Sante, D., Barone, P., Bertacco, R. & Picozzi, S. Electric control of the giant Rashba effect in bulk GeTe. Adv. Mater. 25, 509–513 (2013).
 14.
Zhai, Y. et al. Giant Rashba splitting in 2D organicinorganic halide perovskites measured by transient spectroscopies. Sci. Adv. 3, e1700704 (2017).
 15.
Bawden, L. et al. Hierarchical spinorbital polarization of a giant Rashba system. Sci. Adv. 1, e1500495 (2015).
 16.
Narayan, A. Class of Rashba ferroelectrics in hexagonal semiconductors. Phys. Rev. B 92, 220101 (2015).
 17.
Zhong, Z. et al. Giant switchable Rashba effect in oxide heterostructures. Adv. Mater. Interfaces 2, 1400445 (2015).
 18.
Rodin, A. S. et al. Rashbalike dispersion in buckled square lattices. Phys. Rev. B 96, 115450 (2017).
 19.
Shanavas, K. V., Popović, Z. S. & Satpathy, S. Theoretical model for Rashba spinorbit interaction in d electrons. Phys. Rev. B 90, 165108 (2014).
 20.
Hwang, H. Y. et al. Emergent phenomena at oxide interfaces. Nat. Mater. 11, 103–113 (2012).
 21.
Imada, M., Fujimori, A. & Tokura, Y. Metalinsulator transitions. Rev. Mod. Phys. 70, 1039–1263 (1998).
 22.
Chakhalian, J., Freeland, J. W., Millis, A. J., Panagopoulos, C. & Rondinelli, J. M. Emergent properties in plane view: strong correlations at oxide interfaces. Rev. Mod. Phys. 86, 1189–1202 (2014).
 23.
Ohtomo, A. & Hwang, H. Y. A highmobility electron gas at the LaAlO_{3}/SrTiO_{3} heterointerface. Nature 427, 423–426 (2004).
 24.
Ben Shalom, M., Sachs, M., Rakhmilevitch, D., Palevski, A. & Dagan, Y. Tuning spinorbit coupling and superconductivity at the SrTiO_{3}/LaAlO_{3} interface: a magnetotransport study. Phys. Rev. Lett. 104, 126802 (2010).
 25.
Caviglia, A. D. et al. Tunable Rashba spinorbit interaction at oxide interfaces. Phys. Rev. Lett. 104, 126803 (2010).
 26.
Huang, Z. et al. Interface engineering and emergent phenomena in oxide heterostructures. Adv. Mater. 30, 1802439 (2018).
 27.
Chen, Y. Z. et al. Extreme mobility enhancement of twodimensional electron gases at oxide interfaces by chargetransferinduced modulation doping. Nat. Mater. 14, 801–806 (2015).
 28.
Wang, Y. et al. Roomtemperature giant chargetospin conversion at the SrTiO_{3}–LaAlO_{3} oxide interface. Nano Lett. 17, 7659–7664 (2017).
 29.
Lesne, E. et al. Highly efficient and tunable spintocharge conversion through Rashba coupling at oxide interfaces. Nat. Mater. 15, 1261–1266 (2016).
 30.
Song, Q. et al. Observation of inverse Edelstein effect in Rashbasplit 2DEG between SrTiO_{3}and LaAlO_{3} at room temperature. Sci. Adv. 3, e1602312 (2017).
 31.
Banerjee, S., Erten, O. & Randeria, M. Ferromagnetic exchange, spinorbit coupling and spiral magnetism at the LaAlO_{3}/SrTiO_{3} interface. Nat. Phys. 9, 626–630 (2013).
 32.
Li, X., Liu, W. V. & Balents, L. Spirals and skyrmions in two dimensional oxide heterostructures. Phys. Rev. Lett. 112, 067202 (2014).
 33.
Nakosai, S., Tanaka, Y. & Nagaosa, N. Topological superconductivity in bilayer Rashba system. Phys. Rev. Lett. 108, 147003 (2012).
 34.
Hayden, L. X., Raimondi, R., Flatté, M. E. & Vignale, G. Intrinsic spin Hall effect at asymmetric oxide interfaces: role of transverse wave functions. Phys. Rev. B 88, 075405 (2013).
 35.
Zhong, Z., Xu, P. X. & Kelly, P. J. Polarityinduced oxygen vacancies at LaAlO_{3}∕SrTiO_{3} interfaces. Phys. Rev. B 82, 165127 (2010).
 36.
Alestin, M., Sonu, V. & Tarun Kanti, G. Electrical and thermoelectric transport properties of twodimensional fermionic systems with kcubic spin–orbit coupling. J. Phys. Condens. Matter 29, 465303 (2017).
 37.
Nomura, K., Sinova, J., Sinitsyn, N. A. & MacDonald, A. H. Dependence of the intrinsic spinHall effect on spinorbit interaction character. Phys. Rev. B 72, 165316 (2005).
 38.
Kim, Y., Lutchyn, R. M. & Nayak, C. Origin and transport signatures of spinorbit interactions in one and twodimensional SrTiO_{3}based heterostructures. Phys. Rev. B 87, 245121 (2013).
 39.
Shanavas, K. V. Theoretical study of the cubic Rashba effect at the SrTiO_{3} (001) surfaces. Phys. Rev. B 93, 045108 (2016).
 40.
Zhong, Z., Tóth, A. & Held, K. Theory of spinorbit coupling at LaAlO_{3}/SrTiO_{3} interfaces and SrTiO_{3} surfaces. Phys. Rev. B 87, 161102 (2013).
 41.
Nakamura, H., Koga, T. & Kimura, T. Experimental evidence of cubic Rashba effect in an inversionsymmetric oxide. Phys. Rev. Lett. 108, 206601 (2012).
 42.
Cheng, L. et al. Optical manipulation of Rashba spin–orbit coupling at SrTiO_{3}based oxide interfaces. Nano Lett. 17, 6534–6539 (2017).
 43.
King, P. D. C. et al. Quasiparticle dynamics and spin–orbital texture of the SrTiO_{3} twodimensional electron gas. Nat. Commun. 5, 3414 (2014).
 44.
Nakagawa, N., Hwang, H. Y. & Muller, D. A. Why some interfaces cannot be sharp. Nat. Mater. 5, 204–209 (2006).
 45.
Cancellieri, C. et al. Electrostriction at the LaAlO_{3}/SrTiO_{3} interface. Phys. Rev. Lett. 107, 056102 (2011).
 46.
Warusawithana, M. P. et al. LaAlO_{3} stoichiometry is key to electron liquid formation at LaAlO_{3}/SrTiO_{3} interfaces. Nat. Commun. 4, 2351 (2013).
 47.
Pauli, S. A. et al. Evolution of the interfacial structure of LaAlO_{3} on SrTiO_{3}. Phys. Rev. Lett. 106, 036101 (2011).
 48.
SanchezSantolino, G. et al. Resonant electron tunnelling assisted by charged domain walls in multiferroic tunnel junctions. Nat. Nano 12, 655–662 (2017).
 49.
Spurgeon, S. R., Sushko, P. V., Chambers, S. A. & Comes, R. B. Dynamic interface rearrangement in LaFeO_{3}/nSrTiO3 heterojunctions. Phys. Rev. Mater. 1, 063401 (2017).
 50.
Bergmann, G. Weak localization in thin films: a timeofflight experiment with conduction electrons. Phys. Rep. 107, 1–58 (1984).
 51.
Herranz, G. et al. Engineering twodimensional superconductivity and Rashba spin–orbit coupling in LaAlO_{3}/SrTiO_{3} quantum wells by selective orbital occupancy. Nat. Commun. 6, 6028 (2015).
 52.
Iordanskii, S. V., Lyandageller, Y. B. & Pikus, G. E. Weaklocalization in quantumwells with spinorbit interaction. JETP Lett. 60, 206–211 (1994).
 53.
Knap, W. et al. Weak antilocalization and spin precession in quantum wells. Phys. Rev. B 53, 3912–3924 (1996).
 54.
Kuneš, J. et al. Wien2wannier: from linearized augmented plane waves to maximally localized Wannier functions. Comput. Phys. Commun. 181, 1888–1895 (2010).
 55.
Blaha, P., Schwark, K., Madsen, G. K. H., Kvasnicka, D. & Luitz, J. Wien2K, An Augmented Plane Wave + Local Orbitals Program for Calculating Crystal Properties (ed. Schwarz, K.) (Technische Universität Wien, Vienna, 2001).
 56.
Wang, Z. et al. Anisotropic twodimensional electron gas at SrTiO_{3}(110). Proc. Natl. Acad. Sci. 111, 3933–3937 (2014).
Acknowledgements
L.L. and Z. Z. gratefully acknowledge financial support from the National Key R&D Program of China (2017YFA0303602), 3315 Program of Ningbo, and the National Nature Science Foundation of China (11774360). Calculations were performed at the Supercomputing Center of Ningbo Institute of Materials Technology and Engineering. W. L. and J. C. acknowledge the financial support from the Singapore National Research Foundation under CRP Award No. NRFCRP10201202 and Singapore Ministry of Education MOE2018T22043, AMEIRG180022, A*STAR IAFICP 11801E0036 and MOE Tier 1 FY2018–P23. C.J.L. acknowledges the financial support from the Lee Kuan Yew Postdoctoral Fellowship through the Singapore Ministry of Education Academic Research Fund Tier 1 (Grant No. R284000158114). F. D. and A. M. acknowledge valuable support from KAUST Supercomputing team and some of the fitting calculations were performed on the Phoenix High Performance Computing facility at the American University of the Middle East, Kuwait. W.P. acknowledges partial support of the Tan Chin Tuan Exchange Fellowship in Engineering and Merlion project .The authors would like to acknowledge the Singapore Synchrotron Light Source (SSLS) for providing the facility necessary for conducting the research. The SSLS Laboratory is a National Research Infrastructure under the Singapore National Research Foundation.
Author information
Affiliations
Contributions
W.L., T.W., and Z.Z. conceived and designed the experiments. W.L. performed the samples’ fabrication, transport measurements, and data analysis. L.L. and Z.Z. performed the DFTbased tightbinding calculation. F.D. and A.M. contributed to analyze the magnetotransport data. C.L. and S.J.P. performed STEM experiments. X.Y. performed the XLD experiment. H.R., W.P., B.Z., and Y.L. helped on the structure analyses. W.S.L. and S.W. helped on the samples’ fabrication. W.L., T.W., L.L., and Z.Z. wrote the manuscript and all authors contributed to its final version. T.W., J.C., Z.Z., and A.M. supervised and guided the project.
Corresponding authors
Correspondence to Jingsheng Chen or Zhicheng Zhong or Aurelien Manchon or Tom Wu.
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Peer review information: Nature Communications thanks the anonymous reviewers for their contribution to the peer review of this work. Peer reviewer reports are available.
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Lin, W., Li, L., Doğan, F. et al. Interfacebased tuning of Rashba spinorbit interaction in asymmetric oxide heterostructures with 3d electrons. Nat Commun 10, 3052 (2019). https://doi.org/10.1038/s4146701910961z
Received:
Accepted:
Published:
Further reading

Tailoring magnetic order via atomically stacking 3d/5d electrons to achieve highperformance spintronic devices
Applied Physics Reviews (2020)

Interfacial Control of Ferromagnetism in Ultrathin SrRuO3 Films Sandwiched between Ferroelectric BaTiO3 Layers
ACS Applied Materials & Interfaces (2020)

Spin polarization by firstprinciples relativistic k·p theory: Application to the surface alloys PbAg2 and BiAg2
Physical Review B (2019)

Rashbalike spinorbit and strain effects in tetragonal PbTiO3
Physical Review B (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.